Cast Composite Solid Propellants with Different Combustion ...scindeks- Composite Solid Propellants...
Embed Size (px)
Transcript of Cast Composite Solid Propellants with Different Combustion ...scindeks- Composite Solid Propellants...
Scientific Technical Review, 2015,Vol.65,No.2,pp.3-10 3
UDK: 621.454.019.2:549.514.6 COSATI: 21-09
Cast Composite Solid Propellants with Different Combustion Stabilizers
Vesna Rodi1) Mirjana Dimi1)
Saa Brzi1) Nikola Gligorijevi1)
The effect of four different compounds as the combustion stabilizers of composite solid propellants based on the AP/HTPB/IPDI has been presented in this paper. Except that, various total solid content, ammonium-perchlorate bimodal and trimodal combination of particle sizes ratio have been made by preparing the eleven formulations. For all of them, the burning rate law's parameters and temperature sensitivity, uniaxial mechanical characteristics, apparent viscosity of uncured propellants and physico-chemical and energetic values have been determined and compared.
Key words: composite solid propellant, composite rocket propellant, cast propellant, combustion stability, stabilizers, aluminium, zirconium carbide, titanium oxide, antimony oxide, temperature sensitivity, burning rate.
1) Military Technical Institute (VTI), Ratka Resanovia 1, 11132 Belgrade, SERBIA Correspondence to: Vesna Rodi; e-mail: firstname.lastname@example.org
Introduction OMBUSTION of solid propellants involves a combination of the various ingredients that are consisted
in the cast composite solid propellants (CSP). These ingredients decompose, evaporate and/or pyrolyze, relieving off gases, which then react, resulting in energetic flames that drive the combustion process of the propellant. The instability during the combustion has to be avoided because of many undesirable consequences and can be prevented by adding specific additives . These compounds may have an influence on parameters of all characteristics, especially the ballistic performance and achieving the necessary requirements for the propellant.
The propellant sensitivity to pressure and temperature must be taken into account as well as the influence of the solid component packing (in particular the ratio of different oxidizer fractions) and casting properties. In observed compositions in this paper, ammonium perchlorate (AP) is used as a basic component, whose particle size distribution and fraction ratio significantly affect the way of combustion . For this purpose, all propellant characteristics are necessary to fullfil.
The research results of the CSP including different stabilizer additives will be presented in this paper: - aluminium, Al - zirconium carbide, ZrC - titanium (IV) oxide, TiO2 and - antimony (III) oxide, Sb2O3.
Their influence on the apparent viscosity change of uncured propellant during time, uniaxial mechanical characteristics, physico-chemical and energetic values, burning rate law parameters and calculated temperature sensitivity values of compositions with three different particle size distributions will be tested.
Theoretical part Ammonium perchlorate is the most widely used crystalline
oxidiser in the CSP. It has good characteristics such as good compatibility with other propellant ingredients, good performance, uniformity and availability. Performance can be attributed to the fact that, unlike oxidizers such as potassium nitrate, it is completely convertible to gaseous reaction products [3,4].
Due to its unique characteristic of self-supporting deflagration, the AP combustion has been studied primarily in order to understand the combustion phenomena in the AP-based CSP . It happens that the exothermic decomposition of the AP takes place before melting at temperatures above 200C (270 - 300C). As a basic component, with the largest content, AP significantly affects the way of combustion in these formulations due to specific particle size distribution and fraction ratio.
The burning behavior and flame structure of an AP/HTPB propellant system are influenced by many factors: the chamber pressure, local velocity, AP particle size and mass fraction . The appearance of irregular combustion may occur at a specific particle size distribution of oxidizer powder (the packing density and unfilled space between) and AP/binder ratio. In order to achieve certain requirements and provide good properties, it is necessary to define different combinations of AP particle size distribution of various fractions, total AP and total solid phases content. When the particle size ratio (coarse/fine) is increased up to a level of significant interspace, the burning of fine AP particles will be inhibited by the melting layer of the binder. For the particle size of 20 m, it may be assumed that the AP and HTPB are thermally isolated in the condensed phase. If an energy transfer is allowed between the two segments, the surface
4 RODI,V., DIMI,M., BRZI,S., GLIGORIJEVI,N.: CAST COMPOSITE SOLID PROPELLANTS WITH DIFFERENT COMBUSTION STABILIZERS
temperature of the AP will be reduced, leading to a decrease in the overall burning rate . If there are some compounds taking over the energy transfer to themselves, because of the higher melting points, it is possible to change the combustion process during the form of laminar flow.
The normal burning of CSP produces a burn rate/pressure curve including relatively constant positive slope over the range of expected operating pressures.
The regime thrust, ideally, should be met in all operating conditions, especially in the application temperature range. However, the ballistic properties of propellants show a significant dependence on the external temperature, which affects the operation in a given range.
The combustion of CSP consist of the series of processes. The energetic characteristics and performing rate of these processes determine the propellant burning rate, surface temperature, flame hight and burning surface appearance.
In order to produce a usable propellant formulation, it is necessary to control the burn rate of the propellant, to prevent unacceptable performance (too high or too low pressure) for the intended purpose of the device. The value of temperature sensitivity of the propellant is very important for defining and predicting the ballistic performance and it is expressed as the percent change in burning rate per degree change in the propellant temperature. The first requirement is to obtain a set of burning rate data at various initial temperatures and pressures .
Initial propellant temperature is an important factor of the burning rate level and working regime of the rocket motor, but this influence is unchangeable during motor operation. It is best to take into account the burning rate dependence of the pressure in the chamber for each temperature use.
The collected experimental burning rate data have to be smoothed or fitted. This fitting should be with a minimal disturbance of the natural shape of the burning rate curve. Over the small ranges of pressure, a power law fit in equation (1) may be adequate .
v=B pn (1)
where: v burning rate, p pressure in the chamber, B const. depending on grain temperature and n pressure exponent.
This equation is functional when the change of pressure rate in the chamber is small enough and when the combustion pressure is approximately constant over the entire combustion surface.
Some additives could be added to the propellants in order to modify the burning rate and to maintain the burning rate and temperature sensitivity within acceptable parameters [7,8]. ZrC, Al, TiO2 and Sb2O3 are used for that purpose because of their ability to affect the CSP combustion characteristics: those compounds increase the melted binder viscosity of solid propellant, thereby preventing it to stir with the fine AP. This process enables proper burning at low and high pressures due to the loss of bad burning region in the pressure range . It is important to emphasize that the changing of initial propellants temperature, never modifies the contained chemical energy, but modifies the rate of chemical reactions during propellant combustion . Since almost all missile systems are used in a wide temperature range, it is necessary that solid propellants have the temperature coefficient of the burning rate as small as possible.
Zirconium carbide (ZrC) is an extremely hard refractory
metallic powder with cubic crystal structure. Strong covalent Zr-C bond gives this material a very high melting point (3532C). ZrC powder is shown in Fig.1.
Figure 1. Zirconium carbide powder
Titanium dioxide, (TiO2) or titania, has the melting point at 1843C. It may be found in nature as three minerals and as two high pressure forms, a monoclinic and an orthorhombic. Titania powder is given in Fig.2.
Figure 2. Titania powder
Antimony trioxide is the inorganic, amphoteric compound, with a melting point at 656C. Its structure depends on the temperature. Dimeric Sb4O6 is the gas at 1560C. Antimony trioxide powder is shown in Fig.3.
Figure 3. Antimony trioxide powder
Aluminium is a silvery white, soft metal with a melting point at 660C. This metal is so chemically reactive that native specimens are rare and limited to extremely reducing environments. It is remarkable for the metal's low density and for its ability to resist corrosion due to the phenomenon of passivation with aluminium (III) oxide Al2O3. Aluminium is a universal reductant for CSP, added in the form of the
RODI,V., DIMI,M., BRZI,S., GLIGORIJEVI,N.: CAST COMPOSITE SOLID PROPELLANTS WITH DIFFERENT COMBUSTION STABILIZERS 5
spherical particles with diameter sizes from several up to ten of microns; stirred well with the oxidizer and thus contributes to increase the total energy amount of the active components; the oxidant, which is almost always hygroscopic, is co